#------------------------------------------------------------------------------
#$Date: 2018-01-31 17:20:45 +0200 (Wed, 31 Jan 2018) $
#$Revision: 205967 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/13/2101370.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2101370
loop_
_publ_author_name
'Nakatsuka, A.'
'Yoshiasa, A.'
'Takeno, S.'
_publ_section_title
;
 Site preference of cations and structural variation in
 Y₃Fe~5{-~x}GaₓO₁₂ (0 {łeq} x {łeq} 5)
 solid solutions with garnet structure
;
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              737
_journal_page_last               745
_journal_paper_doi               10.1107/S0108768194014813
_journal_volume                  51
_journal_year                    1995
_chemical_formula_sum            'Fe1.4 Ga3.6 O12 Y3'
_chemical_formula_weight         787.881
_space_group_crystal_system      cubic
_space_group_IT_number           230
_space_group_name_Hall           '-I 4bd 2c 3'
_space_group_name_H-M_alt        'I a -3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.312(2)
_cell_length_b                   12.312(2)
_cell_length_c                   12.312(2)
_cell_volume                     1866.3(5)
_diffrn_radiation_type           Mo
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    32.06
_exptl_crystal_density_diffrn    5.61
_exptl_crystal_F_000             2888
_cod_data_source_file            oh0041.cif
_cod_data_source_block           oh0041g
_cod_original_cell_volume        1866.2(5)
_cod_database_code               2101370
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -y+1/4,x+3/4,z+1/4
3 -x+1/2,-y,z+1/2
4 y+1/4,-x+1/4,z+3/4
5 x,-y,-z+1/2
6 y+1/4,x+3/4,-z+3/4
7 -x+1/2,y,-z
8 -y+1/4,-x+1/4,-z+1/4
9 z,x,y
10 -x+1/4,z+3/4,y+1/4
11 -z+1/2,-x,y+1/2
12 x+1/4,-z+1/4,y+3/4
13 z,-x,-y+1/2
14 x+1/4,z+3/4,-y+3/4
15 -z+1/2,x,-y
16 -x+1/4,-z+1/4,-y+1/4
17 y,z,x
18 y+1/2,-z+1/2,-x
19 z+3/4,y+1/4,-x+1/4
20 -y,z+1/2,-x+1/2
21 -z+1/4,-y+1/4,-x+1/4
22 -y+1/2,-z,x+1/2
23 z+3/4,-y+3/4,x+1/4
24 -z+3/4,y+1/4,x+3/4
25 -x,-y,-z
26 y+3/4,-x+1/4,-z+3/4
27 x+1/2,y,-z+1/2
28 -y+3/4,x+3/4,-z+1/4
29 -x,y,z+1/2
30 -y+3/4,-x+1/4,z+1/4
31 x+1/2,-y,z
32 y+3/4,x+3/4,z+3/4
33 -z,-x,-y
34 x+3/4,-z+1/4,-y+3/4
35 z+1/2,x,-y+1/2
36 -x+3/4,z+3/4,-y+1/4
37 -z,x,y+1/2
38 -x+3/4,-z+1/4,y+1/4
39 z+1/2,-x,y
40 x+3/4,z+3/4,y+3/4
41 -y,-z,-x
42 -y+1/2,z+1/2,x
43 -z+1/4,-y+3/4,x+3/4
44 y,-z+1/2,x+1/2
45 z+3/4,y+3/4,x+3/4
46 y+1/2,z,-x+1/2
47 -z+1/4,y+1/4,-x+3/4
48 z+1/4,-y+3/4,-x+1/4
49 x+1/2,y+1/2,z+1/2
50 -y+3/4,x+1/4,z+3/4
51 -x,-y+1/2,z
52 y+3/4,-x+3/4,z+1/4
53 x+1/2,-y+1/2,-z
54 y+3/4,x+1/4,-z+1/4
55 -x,y+1/2,-z+1/2
56 -y+3/4,-x+3/4,-z+3/4
57 z+1/2,x+1/2,y+1/2
58 -x+3/4,z+1/4,y+3/4
59 -z,-x+1/2,y
60 x+3/4,-z+3/4,y+1/4
61 z+1/2,-x+1/2,-y
62 x+3/4,z+1/4,-y+1/4
63 -z,x+1/2,-y+1/2
64 -x+3/4,-z+3/4,-y+3/4
65 y+1/2,z+1/2,x+1/2
66 y,-z,-x+1/2
67 z+1/4,y+3/4,-x+3/4
68 -y+1/2,z,-x
69 -z+3/4,-y+3/4,-x+3/4
70 -y,-z+1/2,x
71 z+1/4,-y+1/4,x+3/4
72 -z+1/4,y+3/4,x+1/4
73 -x+1/2,-y+1/2,-z+1/2
74 y+1/4,-x+3/4,-z+1/4
75 x,y+1/2,-z
76 -y+1/4,x+1/4,-z+3/4
77 -x+1/2,y+1/2,z
78 -y+1/4,-x+3/4,z+3/4
79 x,-y+1/2,z+1/2
80 y+1/4,x+1/4,z+1/4
81 -z+1/2,-x+1/2,-y+1/2
82 x+1/4,-z+3/4,-y+1/4
83 z,x+1/2,-y
84 -x+1/4,z+1/4,-y+3/4
85 -z+1/2,x+1/2,y
86 -x+1/4,-z+3/4,y+3/4
87 z,-x+1/2,y+1/2
88 x+1/4,z+1/4,y+1/4
89 -y+1/2,-z+1/2,-x+1/2
90 -y,z,x+1/2
91 -z+3/4,-y+1/4,x+1/4
92 y+1/2,-z,x
93 z+1/4,y+1/4,x+1/4
94 y,z+1/2,-x
95 -z+3/4,y+3/4,-x+1/4
96 z+3/4,-y+1/4,-x+3/4
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
Y .125 .0 .25
Fe .0 .0 .0
Fe1 .375 .0 .25
Ga .0 .0 .0
Ga1 .375 .0 .25
O -.0279(3) .0558(3) .1510(3)
